IS : 457 - 1957
CODE OF PRACTICE FOR GENERAL
CONSTRUCTION OF PLAIN AND
REINFORCED CONCRETE FOR DAMS
AND OTHER MASSIVE STRUCTURES
Cement and Concrete Section31 Committee, BDC 2
SHRI E. A. NADIRSHAH The Concrete Association: of Tndia, Bombay. a&
The Institution of Engineers ( India ), Calcutta
SHRI BALESHWAR NATH Central Board of Irrigation & Power ( Miilistry of
Irrigation & Power )
SHRI N. H. BHAGWANANI Engineer-in-Chief’s Branch, Army Headquarters
DR. U. K. BEN&GAL Government Test House. Calcutta
SHRI S. N. M ERJI ( AIlernale)
“5SHRI N. D. DAFTAR Bombay State Road Transport Corporation
DIRECTOR Central Building Research Institute ( Council of
Scientific & Industrial Research ), Roorkee
SHRI C. H. KHADILKM ( AIIcrnale )
SHRI C. L. HANDA Directorate of Designs, Bhakrx Dam, New Delhi
SHRI P. S. BHATNAGAR (./Illivnalf )
DR. H. R. HATTIANGADI The Associated Cement Companies Ltd., Bombay
SHRI V. N. PAI (Alternate)
SHRI P. C. HAZRA Geological Survey of Ind+ Calcutta
DR. R. C. HOON Central Water & Power Commission ( Ministry of
Irrigation & Power)
SHRI GEORGE OOX~EN ( Alkvnate )
SHRI S. B. JOSHI S. B. Joshi & Co., Bombay
SHRI S. R. MEHRA Central Road Research Institute ( Council of Scien-
tific & Industrial Research ). New Delhi
SHRI K. K. NATHA:U Directorate General of Supplies & Disposals
( Ministry of Vorks. Housing & Supply)
MR. E. P. NICOLAIDES Gammon India Ltd., 130mbsy. ctrtd Indian Roads
Congress. New Delhi
REPRESENTATIVE Martin Burn Ltd., Calcutta
SHRI J. M. RIJHWANI Central Public Works Depxtment
SIIRI M. S. HHATIA 4 Akrnate )
SHRI NIHAR CHAXDRA ROY Dalmis Cement ( T%har;it ) I.td.. Calcutta
SHR~ A. K. CHAKRAVARTHI (Alternate)
SnRt SARIJP SINGH National BuiIdin,gs Organization ( hfinistry of
Works, liousmg & Supply)
DEPUTY DIRECTOX ( MATERIAL ) ( .I/tcrw.de )
( Confinztrd on page 2 )
INDIAN STANDARDS INSTITUTION
MANAK BHAVAN, 9 BAHADUR SHAH ZAFAR MARC
NEW DELHI 110002
IS : 457 - 1957
( Contiauad frompage 1 )
SHRI H. P. SINJib Roads Wing, Ministry of Transport
SHRI J. M. TRPHAN ( Alkrnak )
SHRI K. C. !%OD Central Standards Office ( Ministry of Railways )
SHRI S. S. VARMA (Alternate )
DR. LAL C. VBRXAN ( Ex-@cio ) Directer, ISI
SHRI C. S. CHANDRASBKHARA Deputy Director ( Bldg ), ISI
Concrete Subcommittee, BDC 2 : 2
SHRt S. B. Josnr S. B. Joshi & Co., Bombay
SHRI K. F. ANTIA The Associated Cement Companies Ltd., Bombay
SHRI N. H. BHAGWANA... Engineer-in-Chief’s Branch, Army Headquarters
SHRI M. S. BHATIA Central Public Works Department
SHRI T. S. VEDAGIRI ( Ahmate)
DIRICTOR Engineering Research Laboratories, Hyderabad
SHRI P. C. HAZRA Geological Survey of India, Caicutta
DR. R. C. HOON Central Water it Power Commission ( Ministry of
Irrigation & Power )
S~IRIC, L. N. IYENGAR The Concrete Association of India, Bombay
SHRI S. V. NATU Public Works Department, Bombay
SHRI C. C. PATEL ( Alkrnafe )
MR. E. P. NICOLAIDES Gammon India Ltd., Bombay
DR. K. L. RAO Central Water & Power Commission ( Ministry of
Irrigation & Power )
SHRI SARUP SINGH National Buildings Organization ( Ministry of
Works; Housing h Supply)
SIIRI K. RAMA VARYAN ( Altcrnak )
S~IRIH. P. SINHA Roads Wing, Ministry of Transport
SHRI K. C. so00 Central Standards Ofiice ( Ministry of Railways)
IS : 457 - 1957
6. CONSTRUCTIONJOINTS ...
6.1 Location of Joints ...
6.2 Horizontal Joints ...
6.3 Vertlcr.1 Joints ...
6.4 Watertight Joints ...
6.5 Emergemy Joints ...
7. TESTS *.. ...
7.1 Field Tests ...
7.2 Laboratory Test 1::
7.3 Test Records
7.4 Test Pieces ... 1::
7.5 Compression Tests ...
7.6 Flexure Tests
7.7 Failure to Meet Requirements
. . .
. . .
. . .
BETERMINATION OF CONSISTENCYOF CONCRETE BY
VEE-BEE CONSISTOMETERMETHOD... ..:
METHOD OF SECURIN’CHARDENED SPECIMENSOF
CONCRETEFROM THE STRUCTURE ... ...
FLEXURAL STRENGTH OF CONCRETE ( USINGSIMPLE
BEAM WITH THIRD-PWNT LOADING) ...
CODE OF PRACTICE FOR GENERAL .
CONSTRUCTION OF PLAIN AND
REINFORCED CONCRETE FOR DAMS
AND OTHER MASSIVE STRUCTURES
0.1This Indian Standard W;IS adopted by the Indian Standards Institu-
tion on 22 March 1957, on approval by the Building Division Council of
the draft finalized on 14 September 1956, by the Cement and Concrete
0.2 Cement concrete, both plain and reinforted. is being extensively used
in the various multi-purpose projects of the Central Government and irri-
gation and power development schemes sponsored by the States. American
and British practices are being generally followed in the execution of these
works. Indian conditions .differ in many ways from those found in UK
or USA. The Cement and Concrete Sectional Committee felt it desirable
that a code of practice which would take into consideration the variations
obtained under Indian conditions would be a useful guide td engineers
and their technical assistants incharge of such works. This code has been
prepared with this object in view.
0.3 In the preparation of this standard, valuable assistance has bee!
derived from the published materials of the Bureau of Reclamation, Ten-
nessee Valley Authority and the American Society for Testing and
Materials. This assistance is appreciatively acknowledged.
0.4 This standard forms one of a series of Indian Standards on concrete
and reinforced concrete. Other standards in the series are:
*IS: 269-1951 SPECIFICATION POK OKDIN.WY, RAPID-HAKDENING END
Low HUT POKTL.NU CEMEXT
71s: 383-lY52 SPECIFICATION FOH CWKSE AND FINE ACCI~ECATES
FItohfNATURAL SN_JKCESFoK CONCKETE
$ IS: 432-1953 SPECIFIC~ATION FOK MILD STEEL AND HIGIC TENSILE
STEEL BAKS AND HAKD-DK;WN STEEL VIRE FOR CONCKETE RE-
*IS: 455-1953 SPECIFICATION FOR PORTLAND BLAST FUKI.J.~~E SLAG
CEMENT ( Terztativc )
51s: 456-1957 Coce OF PRACTICE FOR PLAIN AND R~~~t;oI~cet) Co,v-
CRETE For< GENEHAL BUILDING CONSTRUCTION ( Raid )
*Third revision in 1976.
Second revision in 1970.
&GXOfld revision in 19&j.
4Secoild revision in 1964.
IS : 457 - 1957
*IS: 515- 1959 SPECIFICATIONFOR NATURAL AND MANUFACTURED
AGGREGATES FOR USE IN MASSCONCRETE
IS: 516-1959METHoDs OF TEST FOR STRENGTH OF CONCHISTE
0.5 This Indian Standard Code requires reference to Indian Standard
Specifications and Codes quoted under 0.4 and also to the following:
71s: 226-1955 SPECIFICATION FOR STRUCTURAL STEEL( Revised )
SlS: 460-1953 SPECIFICATION FOR TEST SIEVES
0.5.1 Wherever a reference to any-Indian Standard mentioned under
0.5, except ~1s: 460-1953, appears in this code of practice, it shall be
taken as a reference to the latest version of the standard.
0.6 In pursuance of the decision of the Government of IJldia to introduce
uniform system of weights and measures throughout the country based
on the metric system, as a first step, wherever possible, metric equivalents
have been given. As the industry gets accustomed to the use of the
metric units, it is intended to drop the foot-pound units altogether from
0.7 For the purpose of deciding whether a particular requirement of this
Standard is complied with, the final value, observed or calculated, expres-
sing the result of a test or analysis, shall be rounded off in accordance with
z IS: 2-1949 Rules for liounrlin~ OH Numerical Values; the nuJnber of
places rdained in the rounded off value should be the same ds t!Jose of
the spccikcl value in the standard.
0.8 lhis code is intended chiefly to lay down requirements regardirlg
quality of material and the JnaJmcr of their use, and. it does not include
all the necessary provisions of a contract.
1.1 This co& covers general construction practices ior plain and rcin-
forced concrete used in dams and other massive structures and a&s pri-
marily at rigid control of concrete work with a view to CJlSUritlg durability,
strength, impermeability and uniformity.
1.1 .l Provisions specified in this code are intended to secure for every
part of tile work homogeneous concrete, which when harderled shall have
the desired proprrties.
1.2 This code requires to be supplemented by special instructions, if any,
for each” job.
t Fifth m-vision in 1975.
18 : 457 - 1957
2.0 For the purpose of this code, the following dcfinitiqns shall a[)&.
2.1 Cement Factor - The weight of cement in kg per cubic metre ( or lb
per 100 cu ft ) of concrete after compaction.
2.2 Concrete -A mixture of Portland cement, water, fine and coarse
aggregates ( and any admixture approved by the engineer-in-charge)
mixed and p~acccl in accordance with the code.
2.3 Consistency -- The relative plasticity of freshly mixed concrete or
mortar, and measure of its workability.
2.4 Cyclopean Aggregates. - Storm of sizes 7.5 to 15 cm C3 to 6 in ).
2.5 Engineer-in-Charge - ‘IIIc Chief Engineer-in-Charge of the watks
or his authorized representative.
2.6 Grout -- A mixture of neat cement and water or cement, sana and
water in fluid state.
2.7 Laitance -- An extremely fine material of little or no hardness which
may collect on the surface of freshly deposited concrete or mortar.
2.5 Mortar - A mixture of Portland cement, fine aggregate and water,
and any admixture approved by the engineer-in-charge.
2.9 Plums -- Large stones over 15 to 23 cm ( or 6 to 9 in ).
2.10 Slump -A measure of consistency in which subsidence of a core
of freshly mixed concrete is determined in accordarice with the method
given in Appendix G of *IS : 456-1057.
2.11 Water-Cement Ratio - The ratio of the weight of water including
surface moisture of aggrcgatrs, to the weight of cemrnt used in the con-
crete mix. This ratio may also be expressed as the number of litres of
water per SO kg ( or gallons of water per 112 lb ) sack of cement.
3.1 Cement - Portland crrncnt and Portlantl bl;tstfurnacc slag cement
usctl for plain ant1 rc*inforcctl concrctc work in dams and other massive
s<ructurrs shall comply rith the requirements of tIS:26Y-1951 and TJh 455
1953, respectively. Special cements may also be spcciticd for use in mass
3.2 Admixture - Admixture, including poztolanas, air entraining agents,
wetting agents, ctc, shall be used onlv under speciiic authorization and
wherever so l~erniittctl, the proportions’and methods of use shall Ge speci-
fied by the engineer-in-charge.
lSccotld revision in 1964.
t Third rwizIoI1 1111976.
IS : 457 _ 1957
3.2J Materials permitted as admixtures shall have established merit
for improving any specific quality of the concrete without causing de-
3.3 Water-Water for mixing concrete, g-rout, or mortar, and also for
washing the aggregates and Curing concrete, shall be clean and free from
injuriWs quantities of acid, alkali, silt, oil, organic matter,.or other im-
3.4.1 Agbqegates for concrete shall conform to @IS: 383-1952 or tIS: 515.
3.4.2 The maximum size of coarse aggregate, as determined by the
biggest square hole through which not less than 95 percent of the aggre-
gate shall pass shall be as large as can be ‘used practicably and econo-
mically under given conditions, but shall be not -larger than any one of
the following :
a) one-fourth the narrowest dimension between the faces of forms,
b) one-third the depth of any slab,
c) three-fourths of the clear space between reinforcement bars, and
d) three-fourths of the narrowest space through which the concrete
shall have to be passed.
3.5 Reinforcement - Reinforcement shall be any of the following:
Mild steel and high tensile steel bars and hard-drawn steel wire
conforming to: IS: 432-1953,
Structural steel sections conforming to 5 IS : 226-1955,
Cold twisted steel bars complying with the requirements of Ap-
pendix A of ?i IS: 456-1957, and
Such other reinforcement as may bc proved suitable, having regard
to the yield point stress, ductility, ultimate resista!lce to tension
and other essential properties of the completed rebforcement as
produced in readiness for use in reinforced concrete.
3.5.1 Mill scale and rust scale, if any, shall be removed from the re-
inforcemen t before use.
3.6 Storaee of Materials
3.6.1 Cement shall be stored in a damp proof place. Handling and
storage facilities shall be such that no cement is stored before use for more
than 120 days counted from the date of despatch by the manufacturer.
lSecmd revision in 1970.
@econd revision in 1966.
$ Fifth revision in 1975.
B Second r&irion h 196+.
IS : 457- 1957
Cement stored beyond 120 days but not exceeding 180 days shall be tested
and rejected if found defective in any way. Cement stored beyond 180
days shall not be used for major construction. Cement shall be ch:ckLd
on the job for contamination or partial setting due to exposure to moisture
3.6.2 Aggregates shall. be stored and handled in such a manper as to
prevent the intermingling of various sizes of aggregates required.separately
for grading purposes. No foreign matter shall be allowed to be mixed up
with the aggregates. Stockpiles shall be built in layers of uniform thick-
3.6.3 Reinforcement shall be stored in such a manner as to minimize
rusting of steel.
4.1 General - The concrete used in dams and other structures may vary
in character from mass concrete having a maximum size of aggregate from
10 cm ( preferahly 15 cm ) to 23 cm [ or 4 in ( ljreferably 6 in ) to 9 in I
and a cement content ranging from about 150 to 235 kg per iu m ( or 250
to 400 lb per cu yd) to heavily reinforced concrete having a maximum
size of aggregate of 2 cm ( or $ in ) and a cement ‘content of approximately
355 kg per cu m ( or 600 lb per cu yd ). To effect the greatest economy,
the concrete should preferably contain the maximum size aggregate S?litdh?
for the place of use and giving the specified strengths.
4.2.1 The proportions of the ingredients in con&ete shaft be detcr-
mined through preliminary laboratory tests on concrete made from re-
presentative samples of ingredients proposed. to be wed in the work. The
tests shall be carried out in accordance iith the procedure described in
Appendix B of *IS: 456-1957. After the water content has been deter-
mined to suit the required consistency, the cement content sl~nll be detei-
mined in the following manner:
A curve representing the relation between water-cement ratio anti
the average compressive strength of concrete at 28 days or earth_,
at which tt)e concrete is to receive its full working load, shall be es-
tablished for a range of values at least 15
cent above 11 times the required strength.
percent below and 15 per-
The curve shall bc fiscd
by at least four pointy, each point rctprescnting the avcragc values of
at least three test specimens. The water-cement ratio to ho adoptctl
on the work shall correspond to that strength on the curve which
is 1) times the strength actually rccpiircd.
*Second rrvisior~ in 1964.
IS : 457 - 1957
The preliminary tests shall be completed well before the beginning of
concreting operations and a complete report on the concrete forming
qualities and Gtability of available aggregates as also recommendations
for their use at the work shah be made and approved by the engineer-in-
charge before actual concreting is started.
4.2.2 No substitutions in the materials used on the work or alterations
in the established proportions shall be made unless additional tests have
been .:onducted to show that the quality and strengths of the resulting
concrete are satisfactory.
4.2.3 The engineer-in-charge may carry out check tests and order
changes in the mix as may be necessary from time to time to maintain
the specified quality of the work. No radical changes, substitutions and
additions in the mix, shall be made without such check tests and subsequent
4.3 Mix Proportions -The proportions of cement, water, aggregates
and other ingredients, if any, necessary to produce concrete of the desired
quality shall be determined as described under 4.2.1. The specified water-
cement ratio shall be strictly adhered to for each class of concrete. Minor
adjustments of the proportions of all ingredients may be made by the
engine&-in-charge in accordance with field tests, specified under 7. Both
the rate and the sequence of pouring shall be strictly regulated as laid down
bv the engineer-in-charge.
4.3.1 Determination of Surface Moisture - In the case of fint? aggre-
gates, the surface moisture shall be determined in accordance with the
method prescribed in Appendix Dof *IS: 456-1957. In the case of coarse
aggregates, percentage of free water shall be determined by weighing a
representative sample, then surface-drying each particle individually with
a clean towel and reweighing the surface-dry sample to determine the
amount of water removed. In calculating the water-cement ratio, the
total weight of water in the mixture including all free water in the aggre-
gate but not including any absorbed moisture, shall be taken into con-
4.4 Workability - As far as possible the concrete shall be of uniform
consistency and quality throughout any pour and for similar parts of the
same structure. However, the consistency and cQ_m.position shall be such
that the concrete can be worked into all corners arid angles of the forms
and that the concrete surrounds completely the reinforcement and em-
bedded metal without causing any segregation of the ingredients or collec-
tion of free water. To this end, the mix may be adjusted slightly aspro-
vided und$r 4.2, if necessary, to provide more workability under specific
conditions, only if no change in the method of either placing or compacting
will accomplish the desired result.
*Swxnd revision in 1964.
IS : 457 - 1957
4.5 Si~lmp ‘.- The !-orltrr,l of concrete under thil; code is based on main-
taining a fGrly unifrirn: k.i~:~!i;i;;t the poirlt of pi:,cement and on holding
the water-remen t ratlo :ib Closely U practicable to the standard ratio
ii&Ymirled ds sy~c~Cifi~:iii:ilci~br4.2.1. LJntlt*rIIOcor:ditions shall the slump
be greater than that rt*cirrirctf to pr.ovl~l~~prof~r pl~~~ernent and compaction
of the fresh concr’ctt~ ;viiilin the forms.
Tlw slump ~XtlnllIY n~cast~rc~din :i(:cordClncc witi. the method prescribed
in Appendix G ot *is: 156 10.57. In the c.ise of wi y small or zero slump,
the consistency shall 1~: IIUCLWW~ 11y the use of Vce-Bee consistometer
described in Appendix .. !-ire allouable slump or consistency shall be
determined by thus ,,!li:il,,,t,r-i:l-ctlar~t,~ and no cll;Lnge in consistency shall
be made vitlr!,rrt his .ti?:~r,>~~~l.
4.4 Measurement of Mater ials
4.6.1 The method of measuring materials for concrete shall be such
that the proportions are controlled and readily checked at any time during
the progress of the irork. Xnterials shall be measured as follows:
Each size of aggregate shall be weighed separately, the cement
and admistures, if sly, shall he weighed in intli5dunl or multipic
batches as approved by the en~irieer-in-cllargc.
4.6.2 WeiPh B&hers .- AI1 we+hine devices shall be subiect to an-
.1 I. I
and weygh hatchers shall meet the following requirements:
The accuracy shall be of the order set for the purpose and shall be
such tllat the indicated weight of any hopprr full of material does
not vary more than one percent from the required weight.
The weighing equipment shall be designed to permit ready and
proper adjustment of the proportions of the m,ix.
The equipment shall be capable of so controlling the rate of de-
livery of each kind and size of materials that the combined in-
accuracy in feeding and measuring during normal operations does
not exceed 3 percent for all aggregates, and 1 percent for water.
The operating mechanism -for measuring the amount of water‘
shall be such that no leakage occurs with the valves closed. The
filling and discharge valves shall not be opened before the IiUing
valve is closed.
e) Test scale weights shall be provided and periodic checks made of
the accuracy of ail weighing equipment.
188.8.131.52 In cases inhere weigh batchers are not available the speci-
fication expressing the mix m proportions of weight should be transformed
into one measuring material by volume. This should be done in the field
*Second revision in 1%
IS : 457- 1957
laboratories attached to each construction site. The co-efficients trans-
forming weight into volume should be determined anew each time the
,aggregate i’s obtained from a different source.
4.6.3 Cement Content-Cement in standard packages or sacks need
not ordinarily be weighed, but shall be periodically checked in the field.
Bulk cement and fractional packages shall be weighed.
4.6.4 Water Content
184.108.40.206 The water-cement ratio established for each class of con-
crete shall be hell within the limits specified under 4.2. The consistency
of the concrete shall be varied only by increasing or by decreasing the
amount of cement paste in each batch.
220.127.116.11 Water for mixing may be measured either by volume or
by weight, and the measuring device shall be accurate to within one per-
cent. A reliable method of compensating for free water shall be used for
maintaining a constant water-cement ratio.
18.104.22.168 Whenever concrete is being conveyed over a long distance
during hot or dry wcathcr, an ahowance may be made for probable eva-
poration during the period concrete is being transported.
4.7.1Machine iMixing at Sire - The mixing of concrete shall be done
in a batch mixer of such approved type as will ensure the homogeneous
distribution of all ingredients. The plant shall be so designed and operated
that ‘all materials entering the mixer including water, can be accurately
proportioned and readily controlled. The entire batch within the mixer
shall be discharged before recharging. The volume of mixed material
per batch shall not exceed the manufacturer’s rated capacity.
22.214.171.124 Method of charging - 171c proper sequence of operations for
the admission of aggregates into any type of mixer shall be ascertained
by trial runs conductecl in order to determine the method giving the best
results. The following sequcncc of charging the mixer may be adopted:
a) Five to ten percent of the total quantity of water required for
mixing, adequate to wet the drum thoroughly, shall be introduced
before the other ingredients m order to prevent any caking of
cement on the blades or sides of the mixers.
b) All dry ingredients ( cement and both fine and coarse aggregates )
shall he simultaneously ribboned into the mixer in such a manner
that the pcrioci of flow for each ingredient is about the same.
IS : 457 - 1957
Eighty to ninety percent of the total quantity of water required for
mixing shall be added uniformly along with the dry ingrcdicnts.
The remaining quantity of water shall be added after all the other
ingredients are in the mixer.
Cobbles or a portion of the coarwst aggregate, howcvcr, may be
added last; tllis facilitates the clcarancc of the chutes and removes
any fine aggrcgrzte or cement adhering to the sides.
126.96.36.199 Time af mixircg
a) Unless othcrvise permitted, machine mixing of each batch shall
continue for not less than the period indicated in Tnljle I. Durlilg
this period the drum shall be rotated at a speed recommended
by the manufacturer. The mixing period shall be timed after all
materials, including water, art in the drum. The efficiency of the
performance of the mixer shall be periodically checked. For any
one mix, the variation in the air-frw wit weights of three samples
taken from the front, centrc and back of a batch of concrete in
the mixer, shall not exceed the following:
For :one batch
Average of 9 batches
37.2 kg per cu m ( or 2.3 lb per cu ft )
Average of 2h, batches
25.9 kg per cu m ( or I.6 lb per cu ft !
19.4 kg per cu m ( or 1.2 lb per cu’ft )
Average of 90 batches 14.6 kg per cu m ( or 0.9 lb per cu ft )
TABLE I TIME OF MIXING
CAPACITY OF MIXER
3 cu m ( or 3 cu yd ) or larger
2 cu m ( or 2 cu yd )
1 cu m (or 1 cu yd ) 0~ smaller
M~~IMIJM 'l‘inm01' MIXING
r--- .____*_...- .. ..~_..._
2 minutes 2! minutes
11 minutes 2 minutes
1f minutes 1 .j miuutes
Each mixer shall have a mechanically oIwratc~t1 timmg device for
signalling tlrc completion of the rccIuired mixing Iwriod. The
actual time of mix+ shall bc checked at least twice during. each
shift and the timing tlcvicc shall be adjusted if in error.
The timing device shall be so interlocked wit11 the discharge gate
of the batch hopper that timing does not start until the discharge
gate is fully closed.and all ingredients are in the drum. .4 suitable
record shall be kept of the average time consumed in charging,
mixing aud discharging a batch during each run.
IS : 457 - 1957
d) Excessive mixing, necessitating the addition of water ko provide
workability shall be avoided.
188.8.131.52 Dischargiltg - The full contents of the drum shall be dis-
charged quickly so as to avoid segregation
184.108.40.206 When the mixer is stopped, before placing again any in-
edients in the mixer all hardened concrete or mortar shall be removed
rom the inner surface of the mixer.
4.7.2 Central Plant Mixing -- Concrete mixing at the central plant
shall be done in accordance with the requirements for machine mixing
at sate ( see 4.7.1 ) before being loaded into the transporting vehicle.
4.7.3 Truck Mixing - Truck mixers, unless otherwise approved, shall
be of the revolving drum type, so constructed that all materials in the
concrete are kept uniformly distributed throughout the mass. The mixer
shall be water-tight when closed. At the proportioning plant, all solid
materials shall be accurately weighed and charged into the drum; the
prescribed quantity of water may either be charged iuto the drum or
measured and placed in the tank meant for carrying the mixing writer.
Trudr mixers shall be provided with some device whereby the time of
hauling, mixing, and introduction of water could be readily checked.
‘4.7.4 Hand Mixing - Hand mixing slrould be avoided in mass con-
crete construction. Hand mixing, if authorized for minor portions of the
work, shall be done on a water-tight platform. The entire mass shall be
turned over using shovels as many times as may be necessary to produce
homogeneous concrete of uniform consistency.
4.7.5 Retemperiq - The retempcring of partially hardened concrete
or mortar requiring renewed mixing, twith or without the addition of cement,
aggregate or water, shall not be permitted.
4.8 Handling and Conveying
4.8.1 The handling and convc,ying of concrete from the mixer to the
place of final deposit shall be dorlc> as rapidly as practicable and without
any objectionable separation or 14~5 of ingredients. Whenever the length
of haul from the mixing plant to the place of deposit is such that the con-
crete unduly compacts or segregates, suitable agitators shall be installed
in the conveying system. Where concrete is being conveyed on chutes
or on belts, the free fall or drop shall be limited to 5 ft ( or 150 cm ) unless
otherwise permitted. The concrete shall be placed in position within
30 minutes of its removal from tlic mixer
is : 457 - 1957
4.8.2 Handliwg Equibmeut
220.127.116.11 Buckets - 13uckets if used, shall be of the bottom-dump
type, permitting an even, controlled flow into the forms or hopper without
undue splashing or segregation. Cars, trucks and skips shall be designed
to facilitate uniform delivery rather than quick dumping.
18.104.22.168 Chutes - Where concrete is conveyed in chutes, the trough
of the chutes shall be of such size and shape as to ensure a steady, uniform
flow of material. The sections shall be made of, .or lined with metal and
al! runs shall have approximately.the same slope, not flatter than 1 vertical
to 2) horizontal. The layout shall be such that the concrete will slide
evenly in a compact mass without any’separation or loss of ingredients.
The required consistency of the concrete.shall not be changed in order to
facilitate chuting. Where it becomes necessary to change the consistency,
the concrete mix shall be completely re-designed. Wherever there is a
free fall within the conveying system, suitable baffle plates, splash boards
or down spouts shall be provided to prevent segregation, splashing, or loss
of ingredients. Wherever it is necessary to hold the discharge end of a
chute more than 300 cm ( or 10 ft ) above the level of the fresh concrete,
a flexible down spout shall be used to break the fall and confine the flow.
The lower end of the spout shall be held close to the place of deposit.
Wherever depositing is intermittent, a discharge hopper shall be provided.
All chutes shall be thoroughly cleaned before and after each run. All
wash water and debris shall,be wasted outside the forms.
22.214.171.124 Pumping - ‘Zhere concrete is permitted to be conveyed
into place by the application of pressure, the pump and piping shall be
suitabty designed and shall be of adequate capacity ior the work. Pumping
shall be permitted only for conveying concrete containing aggregates less
than 7.5 cm ( or 3 in ) maximum size. The operation of the pumping
system shall be such that a continuous streAm of concrete, without air
pockets or interruptions, is delivered. At the end of the run, all concrete
remaining in the pipe line shall be rejected in such a manner as to avoid
any segregation or lack of uniformity. The pump and line shall be
thoroughly cleaned and al! *:;ashwater and debris wasted.
126.96.36.199 Belt conveyors -Where transportation by means of belt
conveyors is permitted, a steady, uniform flow of concrete shall be main-
tained without any segregation or piling up on steep inclines or at transfer
points. The conveyor shall be covered to prevent damage by rain, loss of
heat during cold weather, evaporation or heating by the direct rays of
the sun,,or’other deterioration of the concrete.
Concrete shall not be discharged directly into the forms, unless the
discharge end of the conveyor or pipe can be readily moved about within the
forms so as to place the concrete in even layers as specified under 4.10.2,
IS i 457 - 1957
and 4.10.10. Otherwise, suitable hoppers shall be provided, from which
the concrete shall be dumped in place by means of buckets and short
chutes or spouts.
4.8.3 Cleaning Epipment - At the end of each run and before again
placing any concrete, all hardened concrete or mortar shall be removed
from the inner surface of the conveying equipment. All conveying equip-
ment shall be maintained in good order and kept reasonably free from
deposits of stiff concrete and leakage of mortar.
4.9 Preparation for Placing Concrete
4.9.1 Before depositing any concrete for the ;lexC lift or pour, the
forms Shall not be retightened. The surface of contact shall be allowed
’ to dry out between placing successive lifts of concrete. The top of the
previously deposited concrete shall be thoroughly cleaned and prepared
as specified under 4.10.5.
188.8.131.52 Where new concrete is to be bonded to hard concrete, unless
otherwise ordered and in addition to the requirements specified under
4.105,. the vertical and inclined surfaces which cannot be covered with
mortar shall be given a heavy coat of neat cement grout, vigorously brushed
into all interstices and hollows so as to provide the best possible conditions
for bond and impermeability.
4.9.2 Rock Foundations -- All rock surfaces against which concrete is
to be placed shall be clean and free from mud, dirt, oil, organic deposits,
or other foreign material which may prevent a tight bond between the
rock and concrete. Seams shall be cleaned to a suitable depth and to firm
rock along the side. Where excavation methods or the natural rock strata
do not leave a sufficiently rough surface of contact, the bed shall be
roughened by cutting steps. grooves, trenches, or keyways into the solid
rock. Scaly coatings, hardened grout or concrete, construction debris,
and other objectionable materials shall be removed. Seepage shall be
properly controlled and diverted. The foundation bed and sides shall be
carefully cleaned with stiff brooms, picks, jets of water and air applied
at high velocity or other equally effective means, followed by thorough
washing. After washing and before placing any concrete, water shall be
removed from del’ressions and the rock surface shall be left uniformly
4.9.3 All flat surfaces shall then be coated with mortar about 1.5 cm
( or 4 in ) thick in the case of concrete surfaces and 2 cm ( or 2 in ) thick on
rock surfaces. The water-cement ratio for the mortar layer shall not
exceed that for the regular contrite mixture, and the mortar shall be of
such consistency that it can be spread evenly without flowing. It shall be
IS : 457 - 1957
thoroughly broomed and worked into all irregularities, cracks and crevices.
The manner of spreading and working shall be such as not to cause any
segregation, and concrete shall be placed immediately upon the fresh mortar
before its initial .set.
4.9.4 On very rough or broken surfaces, the first few batches of con-
crete may, if so required, contain only about one-half the regular propor-
tion of coarse aggregate.
4.9.5 No concrete shall be deposited until the foundation has been
inspected and approved. Where the rock is dry enough to absorb water
from the mortar layer, it shall be soaked for at least 24 hours prior to
placing the concrete. Detailed instructions shall be issued for preparing
scaly or cracked foundations requiring special treatment or grouting.
4.9.6 Ear& OY Shale Foundations
184.108.40.206 In the case of earth or shale foundations, all soft or loose
mui and surface debris shall be scraped and removed. The surface shall
be moistened to a depth of about 15 cm ( or 6 in ) to prevent the subgrade
from absorbing water from the fresh concrete. Just before placing the
concrete, the surface of the earth shall be tamped or otherwise consolidated
sufficiently to prevent contamination of concrete during placing. In
general, concrete shall be deposited only upon material lying in a natural,
220.127.116.11 Foundations of porous or free-draining material shall be
thoroughly compacted by flushing and by subsequent tamping or rolling,
if necessary. The finished foundation surface shall then be blanketed with
a layer of tar paper or closely woven burlap carefully lapped and fastened
down along the seams so as to prevent the loss of mortar froni the concrete.
18.104.22.168 Unless otherwise specified, the under-drainage system for
all foundations shall be blanketed as specified under 22.214.171.124.
4.10 Placing Concrete
4.10.1 No concrete shall be placed until the place of deposit has been
thoroughly Inspected and approved, all reinforcement, inserts and em-
bedded metal properly secured in position and checked, and forms thorough-
ly wetted ( except in freezing weather) or oiled. Placing shall be con-
tinued without avoidable interruption while the section is completed or
satisfactory construction joint made.
4,10.2 Within Forms -Concrete shall be systematically deposited in
shallow layers and at such rate as to maintain, until the completion of the
IS : 457 - 1957
unit, a plastic surface approximately horizontal throughout. Each layer
shall be thoroughly compacted before placing the succeeding layer. In
general, the thickness of layers shall not exceed the following limits:
a) Vibrated mass concrete 45 cm (or 18 in)
b) Hand compacted mass concrete 30 cm ( or 12 in )
c) Reinforced concrete 25 cm (or 10 in)
The batches shall be deposited vertically in such a manner as to avoid
segregation, air pockets, or damage to other recently placed concrete.
The concrete shall not be caused to flow or be worked along the forms for
any distance, but shall be compacted as close to the point of deposit as
practicable. Wherever necessary, both the forms and reinforcement
shall be protected against splashing, and all accumulations of partially set,
dried, or caked mortar which may impair the bond or show in the finished
faces shall be removed and wasted before commencing concreting opera-
4.10.3 No concrete shall be deposited at any time except in th
presence of an authorized inspector, nor shall any concrete be placed out-
side regular working hours unless due notification thereof is given in suffi-
cient time to make proper provision for inspection. Wherever concrete is
being deposited at night or under artificial light, both the places of dc-
posit and the mixing and conveying equipment shall be adequately illu-
minated so that all operations are properly observed and inspected.
4.10.4 Temperature of Concrete - When deposited in the forms, con-
crete shall have a temperature of not more than the maximum values as
determined by concrete cooling studies, and appropriate measures shall be
taken to attain this requirement.
all of the following operations:
Such measures may include%ne or
a) Cooling of aggregates by spraying with water and air blasting,
b) Cooling of water used in mixing by refrigeration,
c) USC of cooling towers, and
d) Arranging the placing of concrete during the cooler hours of the
In addition to the above, it may be necessary to control the tcmperaturc
rise of the concrctc after it has been placed by the one or more methods
determined by temperature control studies. All lifts l~lnccd on rock founda-
tion shall not exceed 75 cm ( or 21 ft 1.
4.10.5 Cleaning Joints
126.96.36.199 The joints shall be thoroughly cleaned so as to ex se
sound concrete surfaces. The method shall be by means of jets o4”air
and water applied at high velocity with such additional ro@hcning of the
IS : 457- 1957
surfact?by means of stiff-wire brushes as may be required. Brushing shall
be done by jabbing and digging into the surface rather than by merely
sweeping. The whole process shall be conducted in such manner as not
to loosen the coarse aggregates but vigorously enough to erp&- a fresh
clean-cut concrete surface.
188.8.131.52 Should the next lift be delayed, the contact surface shall
be kept wet and covered so as tr3 minimize the evalmration of curing water
which may cause an injurious coating on the joint. Where necessary all
defective and undesirable concrete shall be removed by chipping and
picking by hand or, if so required, by wet sand blasting the top to a depth
just sufficient to expose a fresh, clean-cut surface over the entire area,
which shall then be thoroughly flushed with water. Every precaution
shall be taken to afford suitable bond for the succeeding lift.
184.108.40.206 Immediately before depositing fresh concrete, the contact
surface shall again be gone over and thoroughly washed to remove all
debris and loose material. The final pick-up of loose materials shall be
made near the centre of the joint and away from the outside edges of the
masonry. Dry contact surfaces shall be kept saturated with water for not
less than 24 hours, but all standing water shall be removed from deprcs-
sions before-spreading the mortar layer. The joint shall then be coveicd
with about 1.5 cm ( or ) in ) of mortar (in the same proportion as in the
original concrete but not lower than 1: 2 ) and the concrete immediately
-deposited thereon according to the manner speciticd under 4.9.2 for rock
220.127.116.11 Hardened surfac1.s of old ITI:IW~W on which new. concrete
is to be placed shall, unless otherwise or&red, be prepared in the same
manner as provided for rock foundations under 4.9.2.
4.10.6 P94eumatic Plmitg - Tht: pneumatic method of placing con-
crete or mortar may IN: used to: sucl1 sj)ecial purposes as tulintl linings,
under-pinning foundations, prcssurc grouting, etc, provided special per-
mission has been granted and the method approved.
4.10.7 Rule 0.fPltrcing --- Concr&ng shall be continued without avoid-
able intcrruptioii until the structure or ycction is complctcd or until satis-
factory construction joints can bc made. Concrctc slinll not bc placed
faster than the placing crew ~a.11 compact it properly. In placing con-
crete in thin mcmbcrs and columns, prccautious shall he taken against too
rapid a placement which may result in movomcnt or fsilurr of the form
due to excessive internal pressure. An interval of at least 4 and prc-
ferably 24 hours should elapse bctwecn the completion of columns alid
walls and the placing of slabs, beams _orgirders supported by them in order
to avoid cracking due to settlement. All concrete shall be placed in ap-
proximately horizont‘al lifts not exceeding 150 cm ( or 5 ft ) in thickilcss
except to expedite the placing of embcddcd materials. The intcl-vx!’
between two lifts shall also be maintained as constant as possible, and
the difference of elevation between any two adjacent blocks shall not be
more than 900 cm ( or 30 ft ) and not less than 150 cm ( or 5 rr 1. A
period of 5 days for 150 cm ( or 5 ft ) of concrete laid shall be allowed
before the next pour unless heat dissipation methods warrant otherwisti.
4.10.8 Placing ‘Plums ’ in Concrete - Where plums are permitted to
be used, they shall be washed and all dripping surface water removed
before being embedded in the concrete. No stone shall be closer than
30 cm ( or 12 in ) to an exposed surface nor nearer than 15 cm ( or 6 in ) to
an adjacent stone. The stones shall not be dropped in place, but each
stone shall be laid and carefully embedded so as.to avoid any injury to the
forms or adjacent masonry and in such a manner that no planes of weak-
ness of unnecessary seams occur in the structure.
4.10.9 Satye Blocks-In placing concrete in large blocks, the work
shall in general proceed from the low side to the high side so that the work-
ing face is never excessively steep nor long. However, for construction
joints in dams, the work shall proceed from the high side to the low side so
as to maintain an upward slope in the downstream direction, unless con-
struction joints are otherwise shown on the drawings. Under no condi-
tion shall the slope be so steep as to cause the concrete to flow without
working, or to cause any segregation. The concrete shall be deposited as
nearly ‘as practicable in final position and shall not be piled up in large
masses at any point and then pushed, shovelled, or vibrated into space
for kJtlg distances. It shall be brought up evenly around all large openings,
conduits, or embedded metal so as to minimize unequal pressure and avoid
dispiacement. For large blocks of concrete in dams and other massive
structures, the sequence and rate of casting successive lifts and adjacent
blocks shall be such as to faciiitate the dissipation of the heat of hydration.
4.10.10 Iirjcctd Coxcyete - A!1 concrete of inferior quality shall be
rejected and removed from ti.c Gt.t: of operations, if possible, before placing
fresh concrctt:; where concrete has rllready been placed, if found inferior,
it shall be dug out and removed from the forms. Any batch, too stiff for
proper placement or in a such condition that it cannot be properly com-
pacted, shall be removed.
4.11.1 .~fethnrl - Concrete shall 1~. thoroughly compacted by means
of suitable tools during and imrncrliately after depositing. The concrete
sIrall 1,~ worked around a11 I-cinforctrment, embedded fixtures, and into
the* corI?c’rs of the forms. Every precaution shall’be taken to keep the re-
inforcctmetlt and embedded metal in proper position and to prevent
IS : 457 - 1957
18.104.22.168 Compacting shall include rodding, spading, tamping,
vibrating, treading, and such other operations except finishing, as are
necessary to consolidate and mould the concrete properly. The rate of
placing mass concrete or reinforced concrete in thin sections. whether
mechanically or by manual labour, shall bc cle,uly defined.
22.214.171.124 Accumulation of water on the surface due to bleeding,
or other causes taking place during compacting shall be stopped as much
as possible by adjustments in the mix. All free water on the surface shall
be removed by sponging or mopping. Under no circumstances shall such
accumulation of water be covered up with concrete, or dry concrete used
to soak up escess water.
126.96.36.199 rJnless otherwise permitted, all concrete shall be com-
pacted by mechanical vibration. The number and type of vibrators shall
be subject to the approval of the engineer-in-charge. In general, only
vibrators of the internal type shall be used. However, in inaccessible
places in the forms where spading, rodding, or forking is impracticabie,
the concrete may be gently Lvorked into place and compacted by light
vibrating or hammering the forms.
188.8.131.52 Wherever practicable, concrete shall be internally vibrated
within the forms, or in the mass, in order to increase the plasticity as to
compact effectively to improve the surface texture and appearance, and to
facilitate placing of the concrete.
184.108.40.206 The intensity and duration of vibration shall be sufficient
to ‘cause complete settlement and compaction without anv stratification
of the successive layers or separation of ingredients. Prehminary experi-
ments in vibrating shall be ‘conducted under actual conditions of mix and
placement in order to determine the optimum duration and method of
vibration, as vc!l as to deveiop the necessary skill.
220.127.116.11 Vibration shall be continued until the entire batch melts
to a uniform appearance and the surface just starts to glisten. -1 minute
film of cement paste shall be discernible between the concrete and the
forms and around the reinforcement. Over vibration causing segregation,
unnecessary bleeding or formation of laitance shall be avoided.
4.11.3 Internal Type Vibrators
18.104.22.168 M,ass concrete sl:a!l be thoroughly compacted with the
aid of high frequency, mechanical vibrators of the internal type, having
IS : 457 - 1957
not less than 3 600 and preferably more than 5 000 impulses per minute.
Immediately after depositing the concrete, the vibrators shall be inserted
into each pile, operated from 10 to 20 seconds in one spot and then moved
to another not over 90 cm ( or 3 ft ) away. The operation shall be re-
peated over until the entire mass is thoroughly compacted and the pile
levelled down. Equal attention shall be paid to the edge of the pile and
to the centre. A sufficient number of two-man vibrators shall be used to
compact each batch properly before placing the next one. A sufficient
number of reserve vibrators in good condition shall be kept on hand at
all times so as to assure that there is no slackening or interruption in com-
22.214.171.124 The USC of flexiblr shaft vibrators, if permitted, shall
closely follow special instructions issud for tt!c purpose.
126.96.36.199 Internal vibrators shall be allowed to penetr;ltcB as deeply
as possible under their own weight and shall so consolidate fhe succcssivc
layers as to break up effectually all- strata or seams. The vibrators shall
be inserted and withdrawn slowly in such manner as not to leave voids in
the plastic concrete. The entire operation shall be condncted in a systr-
matic manner and each course or layer vibrated uniformly. The method
of dumping or depositing the loads shall be so arranged as to keep the
vibrators working continuously during placing operations. The courses
shall be kept approximately l+el, and the concrete. even when depdsited
in thin layers, shall be as st;iI as can be satisfactorily worked. However.
concrete for which a slump greater than 10 cm ( or 4 in ) is specified shall
not be vibrated unless otherwise ordered. Care shall be taken ndt to
disturb a set of partially set layer. The vibrators shall be held vertical
as far as possible.
188.8.131.52 Under no conditions shall internal vibrators strike the face
of the forms, nor shall reinforcement steel or embedded metal be jarred
with sufficient force to impair the bond between the concrete gnd the
4.11.4 Ex&c7nul Tybe Vibmtors
184.108.40.206 Whereyer so required. platform vibrators shall be used
to embed all large stone or cobblblcprojecting above the top of the lift, but
such vibrators shall be used with caution and operated only in such manner
as to avoid pulling exccjs mortar to the surface. The entire top of the lift
for a depth c;i about 30 cm ( or 1 ft ) shall be thoroughly vibrated. Parti-
cular care s.lall be taken in making keyways and shear grooves. Where a
raised key is required, the form shall be filled to overflowing and a plat-
form vibratox used to compact the concrete and bond the key to the body
of the lift.
IS : 457 - 1957
220.127.116.11 Form vibrators shall be permitted-only for special purpose
specified under 18.104.22.168 and extreme care shall be exercised to avoid
pumping air into the concrete.
4.11.5 Surface Voids - Large voids or air pockets, which may be left
in the permanently exposed faces of the structure by vibration, shall be
removed systematically spading the face in the following manner.
Wherever practicable;-a motor-driven, slowly revolving, square steel rod
shall be held in a vertical position and moved slowly back and forth in
short intervals along the entire face. Care shall be taken to avoid prolong-
ing such spading to the point of leaving excess mortar in the face.
4.12 Depositing Concrete Under Water
4.12.1 Concrete shall not be deposited under water, if it is practicable
to unwater the area and place the concrete in the regular manner. If
it is found necessary to deposit any concrete under water, the method,
equipment, materials and mix shall first be approved by the engineer-in-
charge. Concrete shall not be placed in running water.
22.214.171.124 No concrete shall be placed in water colder than 2°C
( or 35°F ). When the water temperature is below 7°C ( or 45°F ), the
temperatrue of the concrete when deposited shall be between 15 to 25°C
(or 60 to 80°F). The difference between the temperature of water and
temperature of concrete shall in no case exceed 5°C ( or 40°F). The
cement content shall be not less than 390 kg of cement per cu m ( or 658 lb
of cement per cu yd) of concrete. The limits for the slump shall be 10 cm
and 18 cm ( or 4 in and 7 in ), the actual slump being decided by the
126.96.36.199 Cofferdams or forms in running water .shall be sufficiently
tight to reduce the velocity of the water to less than 0.3 cu m ( or 10 cu ft )
per minute through the space to be filled with concrete. Cofferdams or
forms in still water shall be sufficiently tight to prevent the loss of mortar.
Pumping or bailing shall not be conducted while the concrete is being de-
posited, and within 24 hours after placing of the concrete.
4.12.2 Methods of Depositing Under Water-Concrete shall be de-
posited continuously until it is brought to the required height. While
&positing, the top surface shall be keGt as nearly level as possible and
the formation of seams shall be avoided. The methods to be used for de-
positing concrete under water shall bc one of the following-
a) Tremie - When concrete is deposited under water by means of a
rremie, the top section of the tremie shall be a hopper large enough
to hold one entire batch of the mix or the entire centents of the
IS : 457 - 1957
transporting bucket when one is used. The trcmic pipe shall be
not less than 20 cm ( or 8 in ) in diameter and shall be large enough
to allow free flow of concrete and strong enough to withstand the
external pressure of the water in which it is suspended, even if a
partial vacuum sl~ould develoij inside the! pipe. Flanged steel
pipe of adequate strength to sustain the greatest length and weight
required for the job should preferably be used. A separate lifting
device shall bc provided for each tremic pipe with its hopper at
the upper end. Unless the rower end of the pipe is equipped with
an approved automatic check valve, the upper end of the pipe shall
be plugged with a wadding of gunny sacking or other approved
material, before delivering the concrete to the tremie pipe through
the hoppei. The plug of sacking or other material is forced out at
the bottom end of the pipe by filling the pipe with concrete. It is
necessary to raise slowly the tremic in order to cause iI uniform
flow of the concrete, but care shall be taken not to empty the
tremie SWthat water enters above the concrete in the pipe. At
all times, .after the placing of concrete is started and until all the
concrete is placed. the lower end of thcbtremip pipe shall be below
the top surface of t!le plastic concrete. This causes the concrete
to build up from below instead of flowing out over the surface and
avoids formation of laitancc layers. If the charge in the tremie is
lost while depositing, the tremic shall be raised above the concrete
surface, and unless sealed by a check valve it shall be re-plugged at
the top end, as at the beginning, before being refilled for depositing
Drop bottom bucket - The top of the bucket shall be open. The
bottom doors shall open freely downward and outward when
tripped. The bucket shall bc filled completely and lowered slowly
to avoid backwash. It shall not be dumped until it rests on the
surface upon which the concrete is to be deposited and when dis-
charged shall be withdrawn slowly until well above the concrete.
4 Bugs - Bags of at least 0.03 cu m ( or 1 cu ft ) capacity of jute or
other coarse cloth shall be filled about two-thirds full of concrete,
the spare end turned under so that bag is square ended and se-
curely tied. They shall be placed carefully in header and stretcher
courses so that the whole mass is interlocked. Bags used for this
purpose.shall be free from deleterious materials.
4.12.3 1‘0 mini&e the formation of laitance, great care shall be
exercised not to disturb the conc.rete while it is being deposited.
4.12.4 If it is necessary iu raise the water after placing the concrete,
the level shall be brought up slowly without creating any waves or com-
motion tending to wash away ctimet;t or to disturb the fresh concrete in
IS : 457 - 1957
4.12.5 Concrete Exposed to Corrosive Water or Soils - Special cements
shall be specified to be used in concrete to be deposited under these condi-
tions. Extreme care shall be taken to secure maximum density and dur-
ability. The placing of any block shall continue without interruption
until the concrete is at least 45 cm ( or 18 in ) above the ground water level.
The corrosive waters or soils shall not touch the concrete during placement
or for at least 72 hours thereafter.
4.13 Weather Conditions
4.13.1 Concrete operations shall be temporarily suspended during
excessively hot, cold, or inclement weather, or whenever conditions are
such that the concrete cannot be properly placed and cured.
4,.13.2 During freezing weather, all aggregates shall be free from ice,
snow, heavy frost and frozen lumps. Whenever the temperature is likely
to fall below -7’C ( or 20°F) within the subsequent 48 hours, concreting
opeiations shal-1 be suspended unless provision has been made to protect
the concrete from freezing. Under such circumstances, the water used for
mixing shall bc heated and the temperature of concrete shall be kept at not
less than 10°C ( or 50°F) for at least 72 hours after placement.
.4.13.3 During hot weather no concrete shall be deposited when the
temperature within the forms is more than 50°C ( or 120°F ). Whenever
ncccssary, exposed surfaces of fresh or green concrete sha!l be shaded from
the direct rays of the sun and protcctedagainst premature setting or drying
by being cured under cortinuous fine spray of water
4.13.4 During continued rainy weather or heavy downpours, all
freshly placed concrete shall hc covrrcd and protected against surface wash.
Special precautions shall bc taken to prevent the formation of lean scams
or sand streaks. Mortar coats for bonding construction joints as speci-
ficd under 4.9.1, 188.8.131.52 and 4.10.5 shall not be placed or left exposed if
the rain is tending to increase the water-cement ratio of the mortar.
Under no conditions shall concrete bc placed in a pool or a sheet of water.
The top of all badly washed or streaked surfaces shall be removed and
wasted bpfore depositing the next course.
4.14 Curing and Protection
4.14.1 All concrete shall be protected against injury. Eqosed
finished surfaces of concrete shall be protected against heating and drying
from the sun for at least 72 hours after placement. Concrete shall, in
general, be kept continuousiy ( not periodically) moist for not less than
14 days. Construction joints shall be cured in the same way as other
1s : 454 - 1957
concrete and shall also, if practicable, be kept moist for at least 72 hours
prior to the placing of additional concrete upon the joint. Horizontal
and approximately horizontal surfaces shall be cured by sprinkling or by
covering with damp sand, or by the use of wet sacks which satisfactorily re-
tain the required amount of water for curing purposes. Where damp
sand or sack cover is used for curing, it shall be completely removed later.
Water curing shall be used ‘on all concrete in dams and shall be applied
by means of sprays or sprinklers to cover the entire area of the concrete.
Forms shall be kept sprinkled until removal. Concrete shall not be dis-
turbed by workmen walking on it or by storing materials on the surface
or otherwise for at least 10 hours after placing.
4.14.2 In special cases, such as powerhouses, the use of an approved,
properly-applied sealing compound on limited areas shall be permitted.
The curing compound shall be of the surface membrance type which shall
thoroughly seal the concrete surface. Curing compound shall not be used
on joints where bonding is required. The concrete surface shall be
thoroughly wetted before applying the compound. All surfaces covered
with curing compound shall be protected from trafhc or injury of the sealing
coat until expiration of the curing period. All methods used for curing
shall leave the concrete free from any discolouration or damage to the
4.15 Repair of Concrete -Repair of all impcrfcctions of the concrete
surfaces necessary to p-~~**pp surfaces that conform to the requirements
shalI be completed as soon = practicable’ after removal of forms and where-
ever possible within 24 hours after tire removal of forms. Fins shall be
neatly removed from surfaces for which finishes F2 and F3 ( see 4.16.2 )
are required. Concrete that is damaged from any cause, and concrete
that is honey-combed, fractured, or otherwise defective, and concrete,
which because of cxccssive surface clepressions, has to be excavated and
built up to bring the surf;lce to the prescribed lines, shall be removed and
replaced with dry-1)atching mortar. Where bulges and abrupt irregu-
larities protrude outside the reqnirecl limits and where it is required to
finish the surfaces with iinishes F2 and F3, the protrusions shall be re-
duced by bush-hammering and grinding so that the surfaces are brought
within the required limits. Drypack filling shalt he used for holes having
at le,ast one surface dimension not greater than the hole depth, for holes
left by removal of fasteners from the ends of ,form tie rods, for grout pipe
recesses, and for narrow slots cut for repair of cracks. Filling of holes
left by the removal of fasteners from the ends of the tie rods in surfaces
for which Fl finish is specified, shall not be required. Dry-patching mortar
shall consist of one part of cement to two parts of sand by volume, and
just enough water to hold the ingredients together. The mortar shall be
placed in layers of 2.5 cm (or 1 in ) each layer thoroughly tamped, an?
the finishing layer shall bc smoothened to form the surface continuous with
IS : 457 - 1957
.the surface of the holes and shall be sound and free from shrinkage cracks
and surrounding concrete. All tilling shall be bonded rightly to the
hollow areas after the fillings have been cured and have dried.
4.16 Finiehea and Finishin@
4.16.1 Concrete surfaces shall be tested where necessary to deter
mine whether surface irregularities are within the specified limits. Surface
irregularities are classified as ‘ abrupt ’ oi *gradual ‘. Offsets caused
by displaced or misplaced form sheathing or lining or form sections, .or
by loose knots in forms or otherwise defective timber forms shall be con-
sidered as abrupt irregularities, and shall be tested by direct measurement.
All other irregularities shall be considered as gradual irregularities, and
tested by use of a template, con&sting of a straight edge or the equivalent
thereof for curved surfaces. The length of the template shall be 150 cm
( or 5 ft ) for testing of formed surfaces and 300 cm ( or 10 ft ) for testing
of unformed surfaces.
4.16.2 Formed Surfaces - The finish for formed concrete surfaces
shall be of the following four classes:
Finish Fl - Finish Fl shall apply to formed surfaces upon which
or against which backfill or concrete is to be placed. The surfaces
require no treatment after removal of forms except removal and
repair of defective concrete and the specified curing. Correction
of surface irregularities shall be done only for depressions which
when measured as described under 4.16.1 exceed 2.5 cm ( or 1 in ).
Finish F2 - Finish F2 shall apply to all permanently exposed
formed surfaces for which finishes F3 and F4 arc not specified.
Surfaces for which finish F2 is specified will need no filling of pits
or sack rubbing and no grinding other than that needed for repair
of surface imperfections. Surface irregularities, measured as
described under 4.16.1 shall not exceed 0.5 cm ( or t in ) for ab-
rupt irregularities and 1 cm ( or 4 in ) for graclual irregularities.
Finish F3 -Immediately after removal of forms from surfaces
designated for F3 finishes, all required patching, clean up and cor-
rection of major imperfections shall bc completed and the surfaces
shall be given a sack-rubbed mortar finish in the following manner:
The surfaces shall be thoroughly wetted and permitted to ap-
proach surface dryness before starting the sack rubbing. The
surfaces shall be finished in areas sufficiently small to prevent com-
plete drying of any part before the sack rubbing is completed for
that area: The mortar usecl for the sack rubbing shall consist
of one pa@ of cement to two parts, by volume, of sand passing
through IS Sieve 100, and enough water so that the consistency
IS . rw - 1957
of the mortar is that of thick cream. The mortar shall be rubbed
thoroughly over the area with clean burlap or a spon_ge rubbed
float, completely filling all pits and irregularities. Wllile the
mix in the 1~01~sis still plastic, a mixture Of the dry ingr~die~~ts of
tilt:mortar in the same proportions shaJ1 he rubbed Over the area.
After the mortar ha5 stiffened adequately to prevent smearing,
but bcforc it llas hartlcned, the exctkss mortar shall he rrrr,Ovcd by
rubbing with clean burlap.
fog spraying shall hc applied
After the final sack rubbing, a ligiir
to the contctl surface, the moisture
th,us applictl being just sufficient to damp the surface without
allowing water to run down the face cl tllc bvalls.
All sack-rubbed arcas shall be kept continuously damp for
at least 72 hours after the final sack rubbing, or until completion
of the curing period for the concrctc. When measured as describ-
cd under 4.16.1, abrupt irrcgularitics shall not exceed 0.5 cm ( or
‘4 in ) for irrcgularitics parallel to thr direction of flow, and 0.25 cm
( or 4 in ) far irregularities in other direction. Gradual irrcgularitics
shall not cxccctl 0.5 cm ( or i in ). Irregularities rxcceding these
limitc< shall hc rcducctl by grinding on a bevc~l of 1 to 20 ratio of
hcigll t to lcq$h.
d) Fiaisll FS - Finish F4 shall apply to formed surfaces where all-
sorptivc form lining is used. Surfaces provided by absorptive form
lining shall not I>(,ruhbcd or trcatcd in any way except for cleaning
by wire IKllshing ant1 grinding off thin fins or small projections.
4.16.3 lJ~$~nzcrl Sur~~tces -The C~CLWSof finish! for unformed con-
crete surfaces arc tlcsign;~trtl by the symbols Ul, U2 and U3. Interior
snrfaccs shall IX, Jop~d for drainage where shown On the drawings. Sur-
faces vhiclI voultl IIC exposed to the weather and, which would normally
be levcbl, sil;dl IX sloped for drainage. Unless the use of otllcr slopes or
level surfaces is spccitied, narrow surfaces, such as tops of walls and curbs,
shall bc sloped approxim;ltely 3 cm per metrc ( or $ in per ft ) of width
border surfaccbs, such as walks, roadways, platforms, and tlecks shall be
sloped approximately 1.5 cm p&r metre ( Or ) in per ft ). The classes of
finish to IX applied shall bc as follows:
a) I;iltish (rl ( screeded finish ) .- shall apply to unformed surtaccs
that are to 1~ covered by backfill or by concretcb and surfaces of
subfloors which will bc cove’red by concrete floor topping. Finish
U1 is also used as tlkc first stagr for Finishes U2 and U3. Finishing
operations shall consist of sufficient levelling and screeding to
produce even uniform surfaces. Surface irregularities, measured
as dcscribcd under 4.16.1 shall not exceed 1 cm ( or ) in ).
b) Finish U2 (jEo&d $nish) - shall’ apply to unformed surlaces
not permanently concealed by backfill or concrete or unformed
surfaces for which Finshcs Ul and U3 are not specified, and shall
IS : 457 - 1957
include floors. of sumps, tops of walls, parking areas, parapet
walls, sdrfaces of gutters, sitlcwalks :md outside entrance slabs.
Finish U2 is also used as the second stngc for Finish U3. Floating
may be performed by use of hand- or power-driven equipment.
Floating shall bc started as soon as the screeded surface has
stiffened sufficiently, and shall IX, tl:c> minimum necessary to pro-
duce a surface that is frc,c from srrcccl marks and is uniform in
texture. If Finish II3 ih to bc al~l~lic~:l,floating shall be continued
until a small amount of mortar itllout excess water is brought
to the surface, so as to permit cffcctivi: trowelling. Surface
irregularities, measured as tlcscribcd under 4.16.1 shallkot exceed
O-5 cm ( or $ in ). Joints and etlgcs of gutters, sidewalks, entrance
slabs, and other joints ant! cclgcs shall be tooled where necessary.
c) Finish U3 ( trowelled jinish ) -- shall apply to unformed surfaces,
such as slabs to be covcrtxtl with built-up roofing or membrane
water-proofing and stair treads. Thcn the floated surface has
hardened suf?iciently to prcvcnt exct’ss of fine material from being
drawn to the surface. steel trowelling shall he started. Steel
trowelling shall be performed with firm pressure, so as to flatten
the sandy texture df the floated surface and produce a dense uni-
form surface, free from blemishes and trowel marks; light steel
trowelling will be permissible on surfaces of slabs to be covered
with built-up roofing or membrane waterproofing, in which light
trowel marks are not considered objectionable. Surface irregu-
larities measured as described under 4.16.1 shall not exceed 0.5 cm
(or & in).
5. FORMS FOR CONCRETE
5.1 General-Forms shall I)r usrd whcrcvrr nrcessary to confine con-
crete and shape it as required. All exposed conrrtstc surfaces having slopes
of one to one or stccpcr shall I)t’ formed, u111css othc;rwist~ clirectcd. Where
the character of the natural material cut into to receive a concrete struc-
ture is such that it can be trimmed to the prcscrihed lines, the use of
forms shall not be r:~cluiretl. The forms sl~all Ilave sufficient strength
and rigidity to hold the concrete ant1 to witllstand the nrcessary pressure,
ramming, and vibration Lvithont excessive deflection from the prescribed
lines. The surfaces of all forms in contact with the concrete shall be clean,
rigid, tight and smooth. Suitable tleviccs shall be used to hold corners,
adjacent ends, and edges of nanels or other forms together in accurate
5.1.1 Metal forms or metal-lined forms shall be permitted for per-
manently exposed surfaces only when an entire surface is to be built
IS : 457 - 1957
completely with such forms. Curved and special forms shall be of a character
that would give smooth concrete surfaces. They shall be so designed and
constructed as not to warp or spring during erection or placing concrete.
Forms to be used more than once shall be maintained in, serviceable condi-
tion, and shall be thoroughly clean and smooth before being Tensed.
Where metal sheets are used for lining forms. thr sheets shall be placed
and maintained on the forms with the minimum amount of wrinkles,
bumps, or other imperfections. The use of sheet m&l tc) correct impcr-
fections in the lining of timber faced forms for surfaces that arc to bt* per-
manently exposed to view shall not be permitted. Vhcre plyvood is used
for form lining, the joints between the sheets shall b(: smooth a11t1as per-
fect as practicable, and no patching of the plywood shall be permitted for
permanently exposed surfaces. Minor imperfections in the plywood shall
be corrected by the use of plastic wood, secured firmly in place and sand-
papered smooth after it has hardened.
5.2 Absorptive Form bng - Absorptive form lining, vhcre directed
to be used, shall be of the type and quality approved l”y the engineer-in-
charge. The form lining shall be highly absorptive to ai:- and water, and
through its absorptive capacity be able to eliminate voids, pits and other
common defects from the concrete surface. The lining shall he readily rc-
movable from the concrete without damage to the surface. It shall pro-
duce a dense co:lcmte surface of uniform and satistactorv texture a:ld
coiour. The lining itself and any treatment employed in its manufactttre
shall not discolour the concrete nor interfere with the IJormal chemical
reaction of the cement. The backing to which absorptive lining is attached
shall be sufficiently smooth, even and free from cracks, knot’ holes, and
other imperfections tci avoid unevenness in the finished surface. The
lining shall be ill sheets of uniform length and kvidth. Location and
direction of the joints shall be approved by the tneitlccr-ill-charge. The
joints between sheets shall be fitted smoothly and accurately. and patching
shall be avoided. Edges shall be brought to light co11tact, tjut shall not be
pressed tightly together. Cutting and trimming shall 1)~ trut: and shall bc
done with tools ~41 adapted to this work so that sharp, smooth, square
edges are produced. Tl~e lining shall be attached to the forms in such a
manner that it is held securely and smoothly in place. Nails or tacks,
if used, shall be spaced in uniform. pattern, and shall be driven flush.
Dents and hammer marks in the surface of the lining shall be avoided.
After the lining has been attached to the form, the joints shall be rubbed
with a smooth tool to press down any projecting fibres. Where absorptive
form lining is in contact with the face of a previous pour, care shall be used
in setting and sufficient pressure shall be applied in tightening form anchors
to produce continuity and evenness at the face, free from offsets, sand
streaks, and other irregularities. The lining shall be kept dry and shall
not be reused.
IS : 457- 1957
5.3 Form Ties -The use of metal rods or other similar devices em-
bedded in the concrete for holding forms shall be permitted if the ends
of the rods are omitted or subsequently removed to a depth of not less
than 5 cm ( or 2 in ) from the surface of the concrete without injury to the
concrete, provided that for walls subjected to water pressure on one side
and required to be watertight, the rods shall not be taken through the
wall. Complete removal of embeddedbds shall not be permissible. Re-
moval of embedded fasteners on the ends of the rods shall be done so as
to leave holes of regular shape for reaming. All holes left by the removal
of fasteners from the ends of the rods shall be immediately reamed with
suitable toothed reamers so as to leave the surfaces of the holes clean and
rough and completely filled with dry patching mortar, and the surface
shall be finished to match the adjacent concrete. U’ire ties shall be per-
mitted only where specifically approved, and shall be cut off fhsh with
the surface of the concrete after the forms are removed. Wire ties shall
not be used where permanently exposed finished surfaces are required.
5.4 Erection of Forms - Before placing concrete, the surfaces of all
forms, except those lined with absorptive form lining, shall be oiled with a
suitable non-staining oil, and, immediately before concrete is placed, pre-
cautions shall be taken to see that all forms are in proper alignment and
that all form anchors and ties are thoroughly secure and tight. Special
care shall be- taken to oil thoroughly the form strips for narrow grooves
so as to prevent swelling of the forms and consequent damage to the con-
crete prior to or during the removal of forms. Where forms for con-
tinuous surfaces are placed in successive units, the forms shall fit tightly
uver the completed surface so as to prevent leakage of mortar from the
concrete and to maintain accurate alignment of the surface. Care shall
be taken to -see that the construction joints formed are smooth, free from
sharp deviations, projections, or edges. Particular attention shall be given
in setting and tightening the form, so that the construction joint surfaces
are plumb and accurately aligned.
5.5 Removal of i!‘wms - Removal of forms shall never be started until
the concrete has thoroughly set and has aged to give it sufficient strength
to carry twice its own wtiight plus the live load which is likely to come
on the structure during the course of construction. The length of time,
the forms would remain in place, shall be decided with reference to weather
conditions, slope and position of the structure or structural member and
the nature and amount of dead and live loads.
55.1 In no case should forms be removed until there is assurance
that their removal is possible without chipping, spalling or defacing the
concrete surface. Furthermore, heavy loads shah not be permitted until
after the concrete has reached its designed strength. All forms shall be
entirely removed from a lift to permit inspection before the forms for
the next lift are set.
IS : 457 - 1957
6. CONSTRUCTION JOINTS
6.1 Location of Joints - The location and type of all construction joints
shall be shown on the drawings, and no other joints or type of joints shall
be built unless specifically approved by the competent authority.
6.2 Horizontal Joints - The stipulations of 4.10.5 for cleaning masonry
joints and bonding nev concrete to old shall apply to all horizontal con-
struction joints. Keyways or dowels for resistance to shear shall be
carefully formed and placed as shown on the drawings. At least 2 hours
shall elal~ after depositing concrete in columns or supporting walls be-
fore placing the concrete in the floor system. All joints shall be finished
to present a sharp level, straight line in the exposed face.
6.3 Vertical Joints-Vertical construction joints shall be built with
essentially the same care as other exposed surfaces. The break between
the adjoining sections of masonry shall be complete, unless otherwise de-
tailed on the drawings.
6.4 Water-tight Joints
6.4.1 Whcrc horizontal construction joints are subject to water pres-
sure, special care shall be taken to bond the next lift of concrete. The
consistency of the concrete shall be carefully controlled so as to avoid sand
streaking; and after compaction no free water shall show anywhere along
the joint. The surface shall be carefully cured as specified under 4.15
and shall IX protcctcd from mechauical injury. Before placing the next
lift, the joint shall hc cleaned and prel)arcd as sljccified under 4.10.5.
6.4.2 In casting vertical joints reqnir’ed to be water-tight, care shall be
taken not to injure or displace the grout pipine vatcr stops, or seals called
for on tile tlrawirlgs.
6.5 Emergency Joints -- Vv’hcrcvcr plncirlg is interrnptctl long enough
for the concrete to take its final set. the working face shall be so formed
and lini~lrctl as to provide union with subscqucnt ,orkequal to that spcci-
fied for regular construction joints.
7.1 Field Tests - Field tests of all concrete being placed shall be re-
gularly conducted. In general, as a reliable indication of other physical
properties, the quality of the concrete being produced shall be judged by a
comparison of the compressive strengths developed within a given period.
IS : 457 - 1957
7.2 Laboratory Test.- A properly equipped testing laboratory to con-
trol the quality of the concrete shall be operated on the work site. The
laboratory shall be fully equipped with apparatus for conductipg all the
usual physical tests for concrete. The compression-testing machme shall
have a capacity of not less than 100 metric tonnes ( or 100 tons ) and shall
be capable of applying the test load at a uniform rate of application.
7.3 Test Records - A complete record shall be kept of all operations.
An accurate daily record shall be made of the location, mix, compressive
strength, water-cement ratio and other physical data pertaining to the
concrete placed in each part of the structure.
7.3.1 The density, durability, imperviousness, generation and loss of
heat, expansion and other physical characteristics of the concrete shall be
tested as often as may be requi;ed to maintain the required properties.
7.4 Test Pieces-In general, not less than one sample shall be taken
from approximately each 380 cu m ( or 500 cu yd ) of mass concrete and
from 190 cu m ( or 250 cu yd) of reinforced concrete placed and for each
class of concrete deposited in any one day’s run. Three cylinders or test
beams shall be made from each sample. The normal number of coutrol
specimens, however, may be changed at the discretion of the engineer-in-
charge. Samples for compression test shall be taken in the field in accor-
dance with Appendix E of *IS : 456-1957. All specimens shall be moulded
immediately after the sample.is taken. They shall be stored in a protected
place under a moist condition at 27 f 2°C ( or 81 f 4°F ) without being
disturbed or moved for at least 24 hours after being zast.
7.4.1 For standard 15 x 30 cm ( or 6 x 12 in ) cylinders, all aggregate
having a maximum dimension of more than 4 cm ( or 14 in ) shall be re-
moved by wet-screening the sample just before moulding the test pieces.
For large cylinders, the maximum size of aggregate left in the sample shall
not be more than one-fourth the diameter of the cylinder. Occasional
specimens as large as can be tested in the field laboratory shall be cast
without removing any aggregate. Such specimens shall be tested to
establish the relation between unscreened and normally screened samples.
The corrective factor thus determined shall be applied to the tested strength
of screened specimens in recording the average daily unit strength of the
concrete placed in the structure.
7.4.2 For dams and other large structures, all field specimens .shall
be finally cured under m&t conditions at a constant temperature of
27 f 2°C ( or 81 f 4°F ) and at 85 percent relative humidity. For small
jobs where a moist room is not available, the specimens shall be cured in
accordance with the standard methodg of making znd storing compression
test specimens in the field.
lSeared revisionin 196%
IS : 457 - 1957
‘i.4.3 Age of Specimeras - kegular tests shall be run at the age of 7
and 28 days, with occasional tests of representative specimens at 14 days
and at 3. 6 and 12 months.
7.5 Compression Tests
7.5.1 For compression tests, the regular size of cylinder and cubes and
the manner of moulding, capping and testing the specimens shall be in
accordance with Appendices B and E of *IS: 456-1957 except that an ap-
proved method of vibration may be used for compacting the concrete.
7.5.2 Wherever required, representative 15 cm ( or 6 in ) cores shall
be drilled from the completed structure and shall be prepared, capped
and tested in accordance with Appendix B. The ultimate compressive
strength and soundness of such specimens shall be compared with the
results of similar fests on standard test cylinders taken from the same run.
7.6 Flexure Tests - For flexure tests, the size and shape of specimens
and the manner of moulding and testing shall be in accordance with Ap-
7.7 Failure to Meet Requirements - Should the test specimens fail
to show the desired uniform quality and characteristics, the directions
given by the engineer-in-charge to improve such concrete, shall be strictly
(Clause 4.5 )
DETERMINATION OF CONSISTENCY OF CONCRETE BY
VEE-BEE CONSISTOMETER METHOD
A-l.1 This appendix deals with the determination of consistency of con-
crete using a V<+Bec Consistometrr, which determines the time required
for transforming, by vibration, a concrete specimen in the shape cf a
conical frustum into a cylinder.
A-2.1 The Vee-Bee Consistometer ( see Fig. 1 ) consists of:
a) A vibrator table resting upon elastic support;
b) ;1 metal pot;
IS : 457 - 1957
c) A sheet metal cone, open at both ends; and
d) A standard iron rod.
A-2.2 The vibrator table ( G ) is 380 mm long and 260 mm wide and is
supported on rubber shock absorbers at a height of about 305 mm above
floor level. Thz table is mounted on a base ( K ) which rests on three
rubber feet, and is equipped with an electricallv operated vibrometer
mounted under it operating on either 65 volts ox 220 volts, three phase,
50 cycles alternating current. A sheet mmtal cone ( B ) open at both ends
is p!aced in the metal pot ( A ) and the metal pot is fixed on to the vibrator
table by means of two wing-nuts (H ). The sheet metal cone is 30 cm
high and its bottom diameter is 20 cm and top diameter 10 cm. A swivel
arm holder ( M ) is fixed to the base and into this is telescoped another
swivel arm ( N ) with funnel ( D ) and guide-sleeve ( E ). The swivel arm
can be readily detached from the vibrating table. The graduated rod
( J ) is fixed on to the swivel arm and at the end of the graduated arm a
Frc.1 VEX-l3m CONSISTOMETER. TYPE VHR
glassdisc ( C ) is screwed. The graduation of the scale on the rod records
the slumps of the concrete cone in ccntimetres and the v&me of concrete
after vibration of the cone in the pot. The standard iron rod is 20 mm
in diameter and 500 mm in length. The electrical equipment mounted
on the base of the consistometer cox,ists of a fixed plug and connector for
IS : 457 - 1957
the electric supply cable, plug and socket contacts for the detachable cable
connected to the vibrometer and a control switc!). A photograph of
the apparatus under operation is given in Fig. 2.
A-3.1A slump test as described in Appendix G of *IS: 456-1957 is per-
formed in the sheet metal cylindrical pot of the consistometer. The glass
2 4 6 8 IO I
FIG.3 RELATION BETWEEN SLUMP IN CM AND VEE-BEE DEGREES
*Second revision in 1964.
IS : 457 - 1957
disc attached to the swivel arm is moved and is placed just on top of the
slump cone in the pot and before the cone is lifted up the position of the
concrete cone is noted by adjusting the glass disc attached to the swivel
arm. ? he cone is then lifted up and the slump is noted on the graduated
rod by lowering the glass disc on top of the concrete cone. The electrical
vibrator is then switched on and the concrete is allowed to spread out in
the pot. The vibration is continued until the whole concrete surface uni-
formly adheres to the glass disc as indicated in Fig. 2 and the time taken
for this to be attained is noted with a stop-watch. The time is recorded in
A-4.1 The consistency of the concrete is expressed
which are equal to the time in seconds under A-3.1.
in Vee-Bee degrees
A-4.2 The required slump is obtained on the basis of the consistency
scale given in Table II.
A-4.2.1 The curve in Fig. 3 indicates the relationship between slump
in cm and the degrees covered by the consistency scale given in Table Il.
TABLE II CONSISTENCY SCALE
NUMDEX OP CHAR.XTERISTICS
40 to 25 to 20
20 to IS to 10
IO to 7 ta c
5 to 4 to 3
3 to 2 to 1
Particles 01 coarse aggregate in the concrete are
adhesive, but concrete does not clot. Risk of
Concrete has the consistency of yery stiff por-
ridge, forms a stiff mound when dumped, and
barely tends to shake or roll itself to form an
almust horizontal surface when conveyed for
a long time in, say, a wheel-barrow
Concrete has the consistency of stiff porridge,
forms a mound when dumped, and shakes or
rolls itself to form a horizontal surface when
conveyed for a long time in, say, a whccl-
Co!xrcte can be shaped into a ball bctwccn the
palms of the hands an? adheres to the skin.
Concrete cannot be rolled int(l a haK1 between
the palms of the hands, but spreads out even
though slowly and without affecting the cohe-
sion of the constituents so that segregation
does not occur.
Concrete spreads uut rapidly and segrcgatlon
JS : 457 - 1957
(Clause 7.5.2 j
METHOD OF SECURING HARDENED SPECIMENS OF
CONCRETE FROM THE STRUCTURE
B-l.1 This method covers the procedure for securing, preparing and
testing specimens of hardened concrete from structures and pavements.
B-2. PRECAUTIONS I
B-2.1 A specimen to be tested for stretlgth shall not be removed from
the structure until the concrete has become hard enough to permit its
removal without disturbing the bond between the mortar and the coarse
aggregate. rn genera1 the concrete shall be 14 days old before the speci-
mens are removed. Specimens that show abnormal defects or that have
been damaged in removal shall not be used.
B-3.1 Core Drill - A core drill shall be used for securing cylindrical core
specimens. For specimens taken perpendicular to a horizontal surface,
a diamond drill shall he used.
B-3.2 Saw -. A saw shall be used for securing beam specimens from
the structure or pavements for flcxural strength tests. The saw shall
have a diamond or silicon carbide cutting edge and shall have adjust-
ments that will permit cutting specimens which conform to the dimensions
prescribed under B-4.2.
B-4.1 Core Specimen - A core specimen for the determination of pave
mrnt thickness shall have a diamet-r of at least 10 cm (or 4 in ). A core
specimen for the determination of compressive strength shall have a dia-
meter at least three times the maximum nominal size of the coarse aggre-
gate used in the concrete, and in no case shall the final diameter of the
specimen be less than twice the maximum nominal size of the coarse aggre.-
gate. The length of the specimen, when capped, shall be, as nearly as
practicable, twice its drameter.
IS : 457 - 1957
B-4.2 Beam Specimen - A bcsm specm~cn for the determination of
flexural strength. in general, shall iia.ve a cross-section of 15 X 15 cm
(or 6 x 6 in ). The specimen shall be at least 53 cm ( or 21 in ) in length
but when two tests for flexural strength are desired for one beam speci-
mzn, it shall be at least 84 cm ( or 33 in ) in length.
NoTE - In mauy ca.&s, particularly with prisms cut from pavement slal=.
the width shall be governed by the size of the coarse aggregate and the depth
hy the thickness ot the slab.
B-5.1 Core Drilling - A core specimen taken perpendicular to a hori-
zontal surface shall bc located, when possible, so that its axis is pcrpendi-
cular to the bed of the concrete as originally placed. A specimen taken
perpendicular to a vertical surface, or perpendicular to a surface with a
batter, shall be taken from near the middle of a unit of deposit. i.e., 380 cu m
( or 500 cu yd ) of mass concrete and from 190 cu m (or 250 cu yd) of re-
inforced concrete placed in any one day’s run.
B-5.2 Slab Removal - A sufficiently large slab shall ‘be removed so
that the desired test spccimcns may be secured without the inclusion of
any concrete whicll has been cracked, spalled, undercut, or otherwise
B-5 3 Beam Sawing - The sawing operation shall be so performed that
the concrete will not bc weakened by shock or by heating. The sawed
surfaces shall bc smooth, plant, parallel. and free from steps, ridges and
growves. Care si~all be taken in handling sawecl beam specimens to avoid
chipping or cracking.
B-6. COMPRESSIVE STRENGTH
B-6.1 End Preparation--Core specimens to be tested in compression
shall have ends that arc essentially smooth. perpendicular to the axis, and
of the same diamctcr as the body of the specimen. The ends of spcci-
mcns wh,ich huvo projections of 0.5 cm ( or b_in ) or more above the normal
plane, or which dcp;Lrt from pcrpcn~licularity to the axis by more than
5 dcgrccs, or whose&uuctcr dcparts.from the me;ln by more than O-25 cm
( or &in ) shall bc salved or tooled until they conform to these tolerances.
B-6.2 Moisture Conditioning - Test specimens shall be completely
submerged in water at room temperature for 40 to 48 hours immediately
prior to the compression test. Specimens shall be tested promptly after
removal from water storage. During the period between removal from
the water storage and testing, the specimens shall be kept moist by covering
with a wet burlap or blanket. They shall be tested in a moist condition.
IS : 457- 1957
B-6.3 CappinB - Before making the compression test, the ends of the
specimen shall he capped in order to meet the requirements given in Ap-
pendix E of IS: 456-1957.
B-6.4 Measurement-Prior to testing, the length of the capl’cd spctci-
men shall be measured to the nearest 0.25 cm ( or 0.1 in j and its average
diamder determined to the nearest 0.25 cm ( or O-1 in ) from two mt*asnrc-
ments taken at right angles near the ccntre of the length.
B-6.5 Calculation and Report - ‘l’hc direction of the npl)lication of
the load with referen& to direction of compaction of the concrctc, in tlie
structure shall he reported. The compressive strength of rach sprscimcm
shall be calculated in kg per ~q cm ( or lb per sq in ) hasetl on ttle average
diameter of the speciinen. If the ratio of lengtll to diamctcr of LIspeci-
men is appreciably less than two, allowance for the ratio of length to diaT
meter shall be made by multiplying the compressive strength hy the ap-
plicable correction factor given in the following table. Values not given
in the table shall be deterinined by interpolation.
RATIO ok LENGTH 0~ STRENGTH CORRECTION
CYLINDER TO DIAMETER FACTOR
( Clause 7.6 )
FLEXURAL STRENGTH OF CONCRETE (USING SIMPLE
BEAM WITH THIRD-POINT LOADING )
C-l.1 This method of test covers the procedurr for determining the
flexural strength of concrete by the use of a simplc~ hram with third-point
C-2.1 The third-point loading method shall be used in making flexurc
tests of concrete employing bearing blocks which sha!l iusure that forces
IS : 457 - 1957
applied to the- beam are vertical only and applied without eccentricity.
A diagram of an apparatus which accomplishes this purpose is shown in
NOTE-Sometimes methods of load application other than the one described
in this appendix are used in the field. If such methods are used, the results should
he correlated with those obtained with the method descrikd in this appendix.
HEAD OF TESTING
OVER FULL WIDTH
BED OF TESTING
Fw.4 DIAGRAMMATIC VIEW OF APPARATUS FOR FLEXURE TEST OF CONCRETE BY THIRD-
POOINT LOADING METHOD
C-2.2 Apparatus for making flexure tests of concrete should be designed
to incorporate the following principles:
a) The distance between supports and points of load application
should remain constant for a given apparatus;
b) The load should be applied normal to the loaded surface of the
beam and in such a manner as to avoid eccentricity of loading;
c) The direction of the reactions shdd be parallel to the direction
of the applied load at all times during the test;
d) The load should bc aeplied at a uniform rate and in such a manner
IS to avtiid shock; and
e) The ratio of distance between point of load application and nearest
reaction to the depth of the beam should be not less than one,
IS : 457 - 1957
C-2.2.1 The directions of loads and reactions may be maintained
parallel by judicious use of linkages, rocker bearings, and flexure plates.
Eccentricity of loading can be avoided by use of spherical or roller bearings.
C-3. TEST SPECIMEN
C-3.1 The test specimen shall have a span as nearly as practicable three
times its depth as tested.
C-4.1 The test specimen shall be turned on its side with respect to its
position as moulded and centred on the bearing blocks. The load-applying
blocks shall be brought in contact with the upper surface at the third point
between the supports. If full contact is not obtained between the speci-
men and the load-applying blocks and the supports, due to the surfaces
of the specimen being out of plane, the surfaces of the specimen where
they are in contact with the blocks or supports shall be capped to meet
the requirements given in Appendix E of*IS: 456-1957. The load may be
applied rapidly up to approximately 50 percent of the breaking load, after
which it shall be applied at such a rate that the increase in extreme fibre
stress does not exceed 10 kg per sq cm ( or 150 lb per sq in ) per minute.
c-5. MEASUREMENT OF SPECIMENS AFTER TEST
ES.1 Measurements to the nearest 0.25 cm ( or O-1 in ) shall be made to
determine the average width and average depth of the specimen at the
section of failure.
C-6.1 If the fracture occurs within the middle third of the span length,
the modulus of rupture shall be calculated as follows:
P = modulus of rupture in kg per sq cm ( or pounds per
square inch ),
R = maximum applied load indicated by the testing machine
in kg (or lb),
= span length in cm ( or in ),
= average width of specimen in cm ( or in ), and
d = average depth of specimen in cm ( or in ).
Non - Weight of the bram ir not included in the above calculation.
*Second revbfoa fu1964.
1s : 457 - 1957
C-6.2 If the fracture occurs outside the middle third of the span length
by not more than 5 percent of the span length, the modulus of rupture
shall be calculated as follows:
R - ?!?_
a = distance between line of fracture and the nearest sup-
port measured along the ccntrc line of the bottom sur-
face of the he:m in cm ( or in.) :LIH~other symbols have
the same significance as given urltlcr C-6.1.
C-6.3 If the fracture occurs outside the middle tltirtl of the span length
by more than 5 percent of the span length, the results of the test shall be
C-7.1 The report shall include the following;
Average width to the nearest 0.25 cm ( or 0.1 in )
Average depth to the nearest 0.25 cm ( or O-1 in ),
Span length in centimetres or inches,
Maximum applied load in kilograms or pounds,
Modulus of rupture calculated to the nearest O-4 kg per sq em
(or 5 lb per sq in ),
iit) Defects in specimen, and
11)Age of specimen.